Home >Documents >Quantum Chemical Modeling of Benzene Ethylation over H-ZSM ... Am Chem Soc 2010 132 11525.pdf ·...

Date post: | 23-Mar-2020 |

Category: | ## Documents |

View: | 0 times |

Download: | 0 times |

Share this document with a friend

Transcript:

Quantum Chemical Modeling of Benzene Ethylation overH-ZSM-5 Approaching Chemical Accuracy: A Hybrid MP2:DFT

Study

Niels Hansen,*,† Torsten Kerber,‡ Joachim Sauer,*,‡ Alexis T. Bell,§ andFrerich J. Keil†

Department of Chemical Engineering, Hamburg UniVersity of Technology,D-21073 Hamburg, Germany, Institut für Chemie, Humboldt-UniVersität zu Berlin,

D-10099 Berlin, Germany, and Department of Chemical Engineering, UniVersity of California,Berkeley, California 94720-1462

Received March 17, 2010; E-mail: [email protected] (N. Hansen); [email protected] (J. Sauer)

Abstract: The alkylation of benzene by ethene over H-ZSM-5 is analyzed by means of a hybrid MP2:DFTscheme. Density functional calculations applying periodic boundary conditions (PBE functional) are combinedwith MP2 energy calculations on a series of cluster models of increasing size which allows extrapolationto the periodic MP2 limit. Basis set truncation errors are estimated by extrapolation of the MP2 energy tothe complete basis set limit. Contributions from higher-order correlation effects are accounted for by CCSD(T)coupled cluster calculations. The sum of all contributions provides the “final estimates” for adsorption energiesand energy barriers. Dispersion contributes significantly to the potential energy surface. As a result, theMP2:DFT potential energy profile is shifted downward compared to the PBE profile. More importantly, thisshift is not the same for reactants and transition structures due to different self-interaction correction errors.The final enthalpies for ethene, benzene, and ethylbenzene adsorption on the Brønsted acid site at 298 Kare -46, -78, and -110 kJ/mol, respectively. The intrinsic enthalpy barriers at 653 K are 117 and 119/94kJ/mol for the one- and two-step alkylation, respectively. Intrinsic rate coefficients calculated by means oftransition state theory are converted to apparent Arrhenius parameters by means of the multicomponentadsorption equilibrium. The simulated apparent activation energy (66 kJ/mol) agrees with experimentaldata (58-76 kJ/mol) within the uncertainty limit of the calculations. Adsorption energies obtained by addinga damped dispersion term to the PBE energies (PBE+D), agree within (7 kJ/mol, with the “final estimates”,except for physisorption (π-complex formation) and chemisorption of ethene (ethoxide formation) for whichthe PBE+D energies are 12.4 and 26.0 kJ/mol, respectively larger than the “final estimates”. For intrinsicenergy barriers, the PBE+D approach does not improve pure PBE results.

1. Introduction

Zeolites are used as catalysts in the petroleum and chemicalindustries to promote a large number of reactions.1,2 For thisreason considerable interest has been devoted in recent yearstoward the development of theoretical models for describingadsorption, diffusion, and reaction in zeolites and toward theclarification of how these processes are affected by zeolitestructure and composition.3,4 The ultimate aim of such work isto simulate the activity and selectivity of zeolite catalysts fromfirst principles. An essential part of this ongoing effort is thedevelopment of accurate methods for the prediction ofthe energies of adsorption/desorption and reaction, as well asthe rate coefficients for these processes.

Density functional theory (DFT) is now routinely applied tocalculate the energy profiles of chemical reactions for systems

as large as zeolites. However, the use of DFT is hampered bythe fact that functionals which can be used efficiently in solid-state simulations do not properly account for long-rangedispersion interactions5,6 and are subject to the self-interactionerror.7,8 This results in underestimated adsorption energies9,10

and energy barriers that are systematically too low,11,12 respec-tively. For noncovalently bonded complexes and large mole-cules13-15 as well as for solid-state and adsorption problems10,16,17

it has been shown that the dispersion interactions can be includedby adding a damped dispersion term as parametrized sum overatom pair C6 contributions (DFT-D).

10,13,14,16,17 Whether thisalso works for processes involving bond rearrangements is a

† Hamburg University of Technology.‡ Humboldt-Universität zu Berlin.§ University of California, Berkeley.

(1) Yilmaz, B.; Müller, U. Top. Catal. 2009, 52, 888–895.(2) Vermeiren, W.; Gilson, J.-P. Top. Catal. 2009, 52, 1131–1161.(3) Smit, B.; Maesen, T. L. M. Chem. ReV. 2008, 108, 4125–4184.(4) Krishna, R. J. Phys. Chem. C 2009, 113, 19756–19781.

(5) Wesolowski, T. A.; Parisel, O.; Ellinger, Y.; Weber, J. J. Phys. Chem.A 1997, 101, 7818–7825.

(6) Zhang, Y.; Pan, W.; Yang, W. J. Chem. Phys. 1997, 107, 7921–7925.(7) Gritsenko, O. V.; Ensing, B.; Schipper, P. R. T.; Baerends, E. J. J.

Phys. Chem. A 2000, 104, 8558–8565.(8) Porezag, D.; Pederson, M. R. J. Chem. Phys. 1995, 102, 9345–9349.(9) Tuma, C.; Sauer, J. Phys. Chem. Chem. Phys. 2006, 8, 3955–3965.

(10) Kerber, T.; Sierka, M.; Sauer, J. J. Comput. Chem. 2008, 29, 2088–2097.

(11) Zhao, Y.; Truhlar, D. G. J. Phys. Chem. A 2005, 109, 5656–5667.(12) Zhao, Y.; Truhlar, D. G. Acc. Chem. Res. 2008, 41, 157–167.

Published on Web 08/02/2010

10.1021/ja102261m 2010 American Chemical Society J. AM. CHEM. SOC. 2010, 132, 11525–11538 9 11525

subject of active research. A further issue with the computationalmodeling of reactions in zeolites is associated with the descrip-tion of the long-range crystal potential and steric effects causedby confinement within the pores of these materials. While theseeffects can be taken into account, in principle, by using largeclusters, such calculations often do not converge with increasingcluster size, suggesting that it would be best to use periodiccalculations.9 The method of choice for correctly including bothlong-range electron correlation as well as the pore topologywould be periodic MP2 calculations. However, for periodicsystems, MP2 calculations are at present only feasible with smallbasis sets and for systems containing only a few atoms in theunit cell.18-20 For accurate calculation of reaction energies andenergy barriers in extended systems, hybrid schemes such asthe MP2:DFT scheme introduced by Tuma and Sauer9,21 canbe applied. This approach combines MP2 calculations withGaussian basis sets for the reaction site and plane-wave DFTfor the full system under periodic boundary conditions. For aseries of cluster models (C) a size-dependent “high-level”correction, defined as the difference between MP2 and DFTenergies is calculated,

and extrapolated to the periodic structure (S). This periodicmodel limit,∆Ẽ(S)high, is added to the plane-wave DFT energyfor the periodic structure, ∆E(S)DFT, to get an estimate of theMP2 energy for the full periodic system,

In eq 2 and throughout this paper we use a tilde to distinguishenergies that were obtained through fitting and/or extrapolationfrom those obtained directly from quantum chemical calculations(MP2, PBE).

This “periodic” MP2 energy, ∆Ẽ(S)MP2, is subsequentlycorrected for errors due to basis set incompleteness, calculatedfor cluster models CCBS, ∆E(CCBS)MP2CBS, as well as for higher-order correlation effects estimated by coupled cluster,CCSD(T), calculations for cluster model CCC, ∆E(CCC)CCSD(T).The final estimate including all of these corrections,∆Ẽ(S)final estimate, is obtained as

The hybrid MP2:DFT approach has been applied previouslyto proton jumps in zeolites,21 adsorption of isobutene9 andstability of tert-butyl carbenium ion22 in zeolite H-FER, and

methylation of alkenes in H-ZSM-5.23 In all cases substantialimprovement regarding the agreement with experimental datawas achieved over pure DFT results.

The hybrid MP2:DFT calculations start with structure opti-mizations and frequency calculations at the DFT level withperiodic boundary conditions. This can be followed by areoptimization on the hybrid MP2:DFT potential energy surfaceusing the high-level correction for an appropriate cluster sizeCOPT according to

This reoptimization has been carried out in refs 9, 21, 22, butis not done in the present study. Here, we follow ref 23 andevaluate the “periodic” MP2 estimate and the final energyestimate according to eqs 2 and 3 as single-point energies atthe DFT optimized structures.

In the present study we employ the MP2:DFT hybrid schemeto revise our previous DFT calculations for the alkylation ofbenzene with ethene over zeolite H-ZSM-5 which used clustermodels of the active site to determine energy barriers and ratecoefficients.24 For the Al12-O20(H)-Si3 site23,25 (numberingaccording to ref 26) we considered both a one-step scheme, inwhich the precursor is represented by coadsorbed ethene andbenzene at the acid site and a two-step mechanism in whichethene is first protonated to form an ethoxide species thatsubsequently reacts with benzene to form the product, ethyl-benzene. The rate coefficients for these elementary steps,together with diffusivities obtained from molecular dynamicssimulations, were then used in a continuum model of a zeolitecrystal to calculate the overall activity as a function of the gas-phase conditions.27 It turned out, however, that the theoreticallydetermined rate coefficients for the one-step mechanism had tobe increased by 2 orders of magnitude to achieve agreementwith experimental data, while the rate coefficients for the two-step mechanism had to be lowered by a factor of 4. Moreover,the apparent activation energy determined for the one-stepmechanism was too low by 15 kJ/mol, while that for the two-step mechanism was slightly higher than the experimentalvalues. It is therefore reasonable to reconsider the alkylation ofbenzene using more sophisticated quantum chemical approachesin order to obtain a clearer view of the energetics and kineticsof this reaction.

The present study has two objectives. The first is to use thehybrid MP2:DFT methodology to calculate accurate intrinsicenergy barriers for the benzene alkylation with ethene and toderive rate coefficients for all elementary steps which are basedon quantum chemical calculations that are converged withrespect to both system size and methodology. The secondobjective is to generate adsorption energies and energy barriersthat can be used as benchmarks in the development ofcomputationally less expensive approaches such as hybrid QM:force field methods25,28,29 or DFT+Dispersion methods.10,13

(13) Grimme, S. J. Comput. Chem. 2006, 27, 1787–1799.(14) Schwabe, T.; Grimme, S. Acc. Chem. Res. 2008, 41, 569–579.(15) Sherrill, C. D.; Takatani, T.; Hohenstein, E. G. J. Phys. Chem. A 2009,

113, 10146–10159.(16) Ortmann, F.; Bechstedt, F.; Schmidt, W. G. Phys. ReV. B 2006, 73,

205101–1/10.(17) Civalleri, B.; Zicovich-Wilson, C. M.; Valenzano, L.; Ugliengo, P.

Cryst. Eng. Commun. 2008, 10, 405–410.(18) Maschio, L.; Usvyat, D.; Manby, F. R.; Casassa, S.; Pisani, C.; Schütz,

M. Phys. ReV. B. 2007, 76, 075101–1/9.(19) Casassa, S.; Halo, M.; Maschio, L.; Roetti, C.; Pisanti, C. Theor. Chem.

Acc. 2007, 117, 781–791.(20) Pisani, C.; Maschio, L.; Casassa, S.; Halo, M.; Schütz, M.; Usvyat,

D. J. Comput. Chem. 2008, 29, 2113–2124.(21) Tuma, C.; Sauer, J. Chem. Phys. Lett. 2004, 387, 388–394.(22) Tuma, C.; Kerber, T.; Sauer, J. Angew. Chem., Int. Ed. 2010, 49, 4678–

4680.

(23) Svelle, S.; Tuma, C.; Rozanska, X.; Kerber, T.; Sauer, J. J. Am. Chem.Soc. 2009, 131, 816–825.

(24) Hansen, N.; Brüggemann, T.; Bell, A. T.; Keil, F. J. J. Phys. Chem.C 2008, 112, 15402–15411.

(25) Clark, L. A.; Sierka, M.; Sauer, J. J. Am. Chem. Soc. 2004, 126, 936–947.

(26) Olson, D. H.; Koktailo, G. T.; Lawton, S. L.; Meier, W. M. J. Phys.Chem. 1981, 85, 2238–2243.

(27) Hansen, N.; Krishna, R.; van Baten, J. M.; Bell, A. T.; Keil, F. J. J.Phys. Chem. C 2009, 113, 235–246.

(28) Clark, L. A.; Sierka, M.; Sauer, J. J. Am. Chem. Soc. 2003, 125, 2136–2141.

∆E(C)high ) ∆E(C)MP2 - ∆E(C)DFT (1)

∆Ẽ(S)MP2 ) ∆E(S)DFT + ∆Ẽ(S)high (2)

∆Ẽ(S)final estimate ) ∆Ẽ(S)MP2 + ∆E(CCBS)MP2CBS +∆E(CCC)CCSD(T) (3)

∆E(S:C)MP2:DFT ) ∆E(S)DFT + ∆E(COPT)high (4)

11526 J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010

A R T I C L E S Hansen et al.

From the different options of the latter,10 we have selected thepragmatic approach of Grimme, adding a parametrized damped1/r6 term to the DFT energy, because it is easy to implementand easy to evaluate with negligible additional computer time,and a clear protocol is available for parameter generation byDFT.13

The elementary processes to which the hybrid MP2:DFTapproach was applied are summarized in Scheme 1. Includedare physical adsorption of ethene, benzene, and ethylbenzenevia π-complex formation with a Brønsted acid site, reactions1-3 in Scheme 1; coadsorption of ethene and benzene on aBrønsted acid site, reaction 4; reaction of ethene with a Brønstedacid site to form an ethoxide species, reaction 5; benzeneadsorption next to the ethoxide species, reaction 6; and etheneadsorption in purely siliceous MFI, reaction 7. Energy barriersand rate coefficients were calculated for the one-step scheme(1s) and for both steps of the two-step mechanism (2s(1) and2s(2); see ref 24 for details).

2. Computational Details

The final estimate adsorption energies and energy barriers werecalculated in three steps. First, a structure optimization for the entireH-ZSM-5 unit cell was carried out using DFT with periodicboundary conditions. Note that in contrast to the original approach9

but following ref 23 hybrid MP2:DFT structure optimization werenot performed because of (i) the computational expense of these

calculations and (ii) the small effect of high-level structurerelaxation effects.9 Second, single-point MP2 and DFT calculationswere conducted on clusters of increasing size cut out from the plane-wave DFT optimized structures to determine the periodic MP2-limit by extrapolation. Third, single-point MP2 calculations withincreasing basis set size are performed to determine the completebasis set limit. Additionally, CCSD(T) calculations on small clustermodels were carried out, to account for higher-order correlationeffects.

2.1. DFT Calculations Applying Periodic Boundary Con-ditions. DFT calculations applying periodic boundary conditionswere performed using the Vienna ab initio simulation program(VASP).30-33 The gradient-corrected exchange-correlation func-tional proposed by Perdew, Burke, and Ernzerhof (PBE)34,35 wasemployed. Plane-wave calculations were conducted using theprojector-augmented wave (PAW) method.36,37 The plane-wavebasis set kinetic energy cutoff was set to 400 eV. Brillouin-zonesampling was restricted to the gamma point. The unit cellparameters R, �, and γ were fixed to 90° in all calculations as nosignificant deviation from the orthorhombic system is expected.38-40

To estimate whether the unit cell vector lengths significantly affectadsorption energies and energy barriers, we calculated theseproperties for some steps using two different sets of cell dimensions.The first set (a ) 20.022 Å, b ) 19.899 Å, c ) 13.383 Å; UC1)comes from crystallographic data,41 while the second set (a )20.157 Å, b ) 20.033 Å, c ) 13.473 Å; UC2) results fromoptimization of an all-silica unit cell as detailed in ref 23. To createan acidic site, one of the 96 Si atoms in the unit cell was replacedby an Al atom in the T12 site25 and the resulting negative chargewas compensated by a proton bonded to one of the neighboringframework oxygen atoms. Specifically the Al12-O20(H)-Si3 site(numbering according to ref 26) was chosen23-25 because of itslocation at the intersection between straight and sinusoidal channels;for details see section S.1 of the Supporting Information.

Minima on the PBE potential energy surface were located usingthe conjugate gradient algorithm with fully relaxed atomic positions.Convergence was considered to be achieved when forces werebelow 10-4 eV/Å. Energies were converged to 10-5 eV in all cases.Transition structures were located by transferring optimized transi-tion structures from our recent cluster study24 into the periodicenvironment and reoptimizing them using the improved-dimermethod.42 Transition structures were considered converged whenforces on all atoms were smaller than 0.05 eV/Å. Stationary pointsfound were characterized by harmonic frequencies obtained bydiagonalization of the full dynamical matrices. The force constantswere obtained by numerical differentiation of forces with a stepsize of 0.02 Å. No scaling factor was applied for the frequencies.DFT energy calculations for gas-phase molecules were carried outusing cubic boxes with edge lengths of 25 Å to minimizeinteractions with the periodic images.23

2.2. MP2 and DFT Cluster Calculations. For the evaluationof the high-level correction (eq 1) single-point energy calculationswere performed on clusters cut out from the plane-wave DFT-

(29) De Moor, B. A.; Reyniers, M.-F.; Sierka, M.; Sauer, J.; Marin, G. B.J. Phys. Chem. C 2008, 112, 11796–11812.

(30) Kresse, G.; Hafner, J. Phys. ReV. B 1993, 48, 13115–13126.(31) Kresse, G.; Hafner, J. Phys. ReV. B 1994, 49, 14251–14296.(32) Kresse, G.; Furthmüller, J. J. Comput. Mater. Sci. 1996, 6, 15–50.(33) Kresse, G.; Furthmüller, J. Phys. ReV. B 1996, 54, 11169–11186.(34) Perdew, J. P.; Burke, K.; Ernzerhof, M. Phys. ReV. Lett. 1996, 77,

3865–3868.(35) Perdew, J. P.; Burke, K.; Ernzerhof, M. Phys. ReV. Lett. 1997, 78,

1396.(36) Blöchl, P. E. Phys. ReV. B 1994, 50, 17953–17979.(37) Kresse, G.; Joubert, D. Phys. ReV. B 1999, 59, 1758–1775.(38) Hay, D. G.; Jaeger, H.; West, G. W. J. Phys. Chem. 1985, 89, 1070–

1072.(39) van Koningsveld, H.; Jansen, J. C.; van Bekkum, H. Zeolites 1987, 7,

564–568.(40) van Koningsveld, H. Acta Crystallogr. 1990, B46, 731–735.(41) van Koningsveld, H. Acta Crystallogr. 1987, B43, 127–132.(42) Heyden, A.; Bell, A. T.; Keil, F. J. J. Chem. Phys. 2005, 123, 224101–

1/14.

Scheme 1. Elementary Processes Involved in the Alkylation ofBenzene with Ethene

J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010 11527

Modeling of Benzene Ethylation over H-ZSM-5 A R T I C L E S

optimized periodic structures. A series of 16 cluster models ofincreasing size was constructed for all stationary points with thelargest cluster containing 30 T-atoms. The cluster models weresaturated with hydrogen atoms such that the terminating groupswere SiO-H (r(O-H) ) 0.967 Å) or AlO-H (r(O-H) ) 0.963 Å).43Figure 1 shows adsorbed ethylbenzene as an example for the largestsystem considered.

For each cluster model and gas phase molecule, MP2 energieswere computed with the TURBOMOLE program package44-46

using basis sets of triple-� quality.47 For carbon atoms and thoseoxygen atoms which connect two T-atoms (T-O-T) the TZVPPbasis set was chosen while for all other atoms the TZVP basis setwas used. Following Tuma and Sauer9 we denote this combinationas TZVP(P) in the remainder of this paper. Electrons in molecularorbitals corresponding to C 1s, O 1s, Al 1s, and Si 1s atomic orbitalswere excluded from the MP2 correlation scheme.

DFT energies for each cluster model and gas-phase moleculewere computed within the RI approximation48-50 using the PBEfunctional34,35 and a basis set of quadruple-� quality (def2-QZVP).51

Energies were not corrected for BSSE which is expected to benegligible for this basis set. The employment of Gaussian typeorbitals (GTO) as basis sets for this part of the hybrid method differsfrom previous studies where the PBE energies for all cluster modelshave been obtained with the same plane-wave methodology as wasused for the periodic structure.9,23 Comparison of adsorptionenergies for ethene adsorption on the acid site for several clustermodels showed energy differences below 0.5 kJ/mol between bothapproaches.

The differences between MP2 and PBE adsorption energiesconverge monotonically with the cluster size Cn (see below) and

can be extrapolated to the periodic limit using the followinganalytical expression:9

It consists of an additive constant, Eadd, which accounts for all effectscontributing to MP2-PBE adsorption energy differences that do notstrongly depend on the cluster size, for example the self-interactioncorrection (SIC) error, and a term

which has the analytical form of a sum over damped atomic C6dispersion contributions for all atom pairs i and j at distance Rij.Nn denotes the number of atoms in cluster Cn. For the dampingfunction fd(Rij) we use the functional form and the parameter valuesproposed by Grimme.13 The global scaling parameter, s6, dependson the particular exchange-correlation functional. For the PBEfunctional its value is 0.75.13 The five atomic C6 coefficients, C6i ,and the additional constant, Eadd, are fitted for each reactionindividually by minimizing

using a series of nmax cluster models Cn of increasing size. Theparameters obtained are given in Table S.6 of the SupportingInformation. Using the fitted C6 parameters,Edisp(S)is obtained byapplying eq 6 to the periodic structure by means of lattice sums.10

The high-level correction for the periodic system S,

has then to be added to the periodic DFT result, ∆E(S)PBE, to getestimates for the full “periodic” MP2 adsorption energies,∆Ẽ(S)MP2that has been introduced in eq 2.

The same procedure is applied to the apparent energy barrierswhich also show a monotonic decay. They are fitted according toeq 7 and extrapolated to the periodic limit. The fit parametersobtained are given in Table S.7 of the Supporting Information. Incontrast, the high-level corrections for the intrinsic barriers havebeen obtained as difference of the high-level corrections of theapparent barriers and the respective adsorbate complexes. As shownin section S.7 of the Supporting Information, the differencesbetween MP2 and PBE results for the intrinsic energy barriersdepend only weakly on the cluster size and do not show a monotonicdecay with increasing cluster size which makes fitting and directextrapolation less reliable.

2.3. Complete Basis Set Extrapolation. The incompletenessof Gaussian basis sets introduces an error in the MP2 calculationsthat can be accounted for approximately by extrapolation to thecomplete basis set (CBS) limit. BSSE-corrected52 RI-MP2 single-point energies obtained using Dunning’s correlation consistentpolarized valence triple-� and quadruple-� basis sets cc-pVXZ (X) 3 and 4)53,54 were used for this purpose. Extrapolation to theCBS limit assumes an exponential behavior of the Hartree-Fockenergy and an X-3 behavior of the correlation energy as a functionof the basis set cardinal number X ()3,4), see section S.2 of theSupporting Information for more details.

The CBS limit correction,∆E(CCBS)MP2CBS,

(43) Sierka, M.; Sauer, J. Faraday Discuss. 1997, 106, 41–62.(44) Ahlrichs, R.; Bär, M.; Häser, M.; Horn, H.; Kölmel, C. Chem. Phys.

Lett. 1989, 162, 165–169.(45) Hättig, C. J. Chem. Phys. 2003, 118, 7751–7761.(46) Hättig, C.; Hellweg, A.; Köhn, A. Phys. Chem. Chem. Phys. 2006, 8,

1159–1169.(47) Schäfer, A.; Huber, C.; Ahlrichs, R. J. Chem. Phys. 1994, 100, 5829–

5835.(48) Eichkorn, K.; Treutler, O.; Öhm, H.; Häser, M.; Ahlrichs, R. Chem.

Phys. Lett. 1995, 240, 283–290.(49) Eichkorn, K.; Treutler, O.; Öhm, H.; Häser, M.; Ahlrichs, R. Chem.

Phys. Lett. 1995, 242, 652–660.(50) Eichkorn, K.; Weigend, F.; Treutler, O.; Ahlrichs, R. Theor. Chem.

Acc. 1997, 97, 119–124.(51) Weigend, F.; Furche, F.; Ahlrichs, R. J. Chem. Phys. 2003, 119, 12753–

12762.

(52) Boys, S. F.; Bernardi, F. Mol. Phys. 1970, 19, 553–566.(53) Dunning, T. H. J. Chem. Phys. 1989, 90, 1007–1023.(54) Woon, D. E.; Dunning, T. H. J. Chem. Phys. 1993, 98, 1358–1371.

Figure 1. The largest system calculated with MP2/TZVP(P) in the presentwork is the 30T cluster with the overall composition C8H53O81Si29Al (here:adsorbed ethylbenzene, viewed along the straight channel). Color codes:oxygen (red), silicon (yellow), aluminum (pink), hydrogen (white), carbon(gray).

EHL-corrfit (n) ) Edisp(n) + Eadd (5)

Edisp(n) ) -s6 ∑i

Nn-1

∑j)i+1

Nn √C6i · C6jRij

6fd(Rij) (6)

∆({C6i }, Eadd) ) ∑

n)1

nmax

[(∆E(n)MP2 - ∆E(n)PBE) - EHL-corrfit (n)]2

(7)

∆Ẽ(S)high ) ∆Ẽ(S)MP2 - ∆E(S)PBE ≈ Edisp(S) + Eadd(8)

11528 J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010

A R T I C L E S Hansen et al.

is the difference between BSSE-corrected adsorption energiesextrapolated to the complete basis set limit and BSSE-uncorrectedadsorption energies obtained with the TZVP(P) basis set calculatedfor cluster model CCBS. ∆E(CCBS)MP2CBS is added to ∆Ẽ(S)MP2 obtainedfrom eq 8 to get a BSSE-free MP2 adsorption energy for theperiodic structure. For CCBS we adopt the T18 cluster model, exceptfor the coadsorption of ethene and benzene for which the T16 clusteris adopted because of the high computational costs associated witha 3-body counter-poise correction. In section S.2 of the SupportingInformation we show that from the 16T-18T size region on, theCBS limit correction can be assumed constant.

The CBS limit corrections for intrinsic energy barriers wereobtained indirectly from the CBS limit corrections of the apparentenergy barriers and those of the associated adsorbate complex.

2.4. CCSD(T) Calculations. The reliability of MP2 to predictadsorption energies and energy barriers for the alkylation wasassessed by performing single-point CCSD(T) calculations for allstationary points on a modified 3T cluster model. This modifiedmodel was obtained from the 3T model used in the cluster seriescalculations by replacement of SiO-H by Si-H terminations witha Si-H bond length of 1.455 Å23 (see Figure 2) to reduce thecomputational expenses. In section S.4 of the Supporting Informa-tion we show, by evaluating MP2/CBS-PBE+D energies as functionof the cluster size, that higher-order correlation effects depend onlyweakly on the cluster size, leading us to conclude that a relativelysmall cluster model is sufficient. The CCSD(T) calculations werecarried out with the MOLPRO code55 employing Ahlrich’simproved triple-� valence basis set (def2-TZVP)56 for all atoms.For our final estimates of adsorption energies and energy barrierswe add the difference between CCSD(T) and RI-MP2 adsorptionenergies and energy barriers calculated on the same 3T cluster,∆E(C3)CCSD(T), to the “periodic” MP2 adsorption energies andenergy barriers.

2.5. PBE+D//PBE Calculations. With PBE+D//PBE we denotethe evaluation of the energy of plane-wave DFT-optimized struc-tures according to

with the dispersion term given in eq 6 using the transferable C6-coefficients of Grimme.13 Adsorption energies calculated in thisway still contain the self-interaction error but are significantly lessexpensive to obtain than those determined from the full MP2:DFTcalculation because eq 6 can be applied directly to the periodicunit cell optimized by plane-wave DFT. By doing so the compu-tationally expensive determination of MP2 and DFT adsorptionenergies for a series of clusters as well as the basis set limitextrapolation procedure are avoided. It is therefore of great interestto evaluate further the transferability of the C6-coefficients publishedby Grimme13 to solid state and surface problems.10

2.6. Calculation of Intrinsic Rate Coefficients. Intrinsic ratecoefficients are calculated from conventional transition statetheory,57,58

where kB is Boltzmann’s constant, h is Planck’s constant, T is theabsolute temperature, and Eqis the difference in electronic energies

between the transition state and the reactant state. With σ we denotea reaction path symmetry number,59 while QTS and QR are thepartition functions of the transition state and the reactant state,respectively. The most straightforward method to calculate thepartition functions is to assume immobile adsorption, that is, acomplete conversion of frustrated rotational and translationaldegrees of freedom into vibrations. However, contributions fromlow vibrational modes corresponding to rotational and translationalmovements of adsorbate molecules are often not adequately takeninto account by this treatment60 and may lead to an underestimationof the partition function. As is shown in section S.5 of theSupporting Information, the assumption of immobile adsorption isa reasonable approximation for both the one-step mechanism andthe elementary steps of the two-step mechanism.

3. Results and Discussion

3.1. Adsorption of Reactants and Products. 3.1.1. PeriodicDFT Structure Optimization. The first row of Table 1 showsthe PBE interaction energies for all adsorbate molecules obtainedwith the UC1 set of cell parameters. The size of the unit cellaffects the physisorption energies by up to 5 kJ/mol (see sectionS.6.1 of the Supporting Information for a detailed discussion).The orientation of all adsorbates within the unit cell is shownin Figure 3. The absence of imaginary frequencies confirmedthat all stationary points were true minima. The zero-pointvibrational energies calculated from these PBE frequencies arealso shown in Table 1 (seventh row). The calculated wavenum-ber for the O-H stretching mode is 3705 cm-1 (H on O20) ingood agreement with other theoretical studies on H-FER (3680cm-1)61 and H-MOR (3709 cm-1)62 employing similar planewave calculations. A change in the unit cell parameters affectsthe O-H stretching mode by just 4 cm-1. The calculatedfrequencies are larger than the experimental wave numbers of3623 cm-1 (at 170 K)63 and 3612 cm-1 (at 300 K),63,64 asexpected, due to the limited accuracy of harmonic DFT forceconstants and neglect of anharmonicities. The calculated red-shifts of the O-H stretching modes induced by adsorption ofethene and benzene, -535 cm-1 and -498 cm-1, respectively,

(55) Werner, H.-J.; et al. MOLPRO: A package of ab initio programs,version 2006.1; Cardiff: UK, 2006.

(56) Weigend, F.; Ahlrichs, R. Phys. Chem. Chem. Phys. 2005, 7, 3297–3305.

(57) Eyring, H. J. Chem. Phys. 1935, 3, 107–115.(58) Evans, M. G.; Polanyi, M. Trans. Faraday Soc. 1935, 31, 875–894.

(59) Fernándes-Ramos, A.; Ellington, B. A.; Meana-Pañeda, R.; Marques,J. M. C.; Truhlar, D. G. Theor. Chem. Acc. 2007, 118, 813–826.

(60) De Moor, B. A.; Reyniers, M.-F.; Marin, G. B. Phys. Chem. Chem.Phys. 2009, 11, 2939–2958.

(61) Tuma, C. A QM/QM hybrid method for MP2/plane-wave-DFT studiesof extended systems. Ph.D. Thesis Humboldt-Universität Berlin, 2006.

(62) Bučko, T.; Benco, L.; Demuth, T.; Hafner, J. J. Chem. Phys. 2002,117, 7295–7305.

(63) Trombetta, M.; Armaroli, T.; Gutierrez Alejandre, A.; Ramirez Solis,J.; Busca, G. Appl. Catal., A 2000, 192, 125–136.

(64) Zecchina, A.; Spoto, G.; Bordiga, S. Phys. Chem. Chem. Phys. 2005,7, 1627–1642.

∆E(CCBS)MP2CBS ) (∆E(CCBS)HFCBS + ∆E(CCBS)corrCBS) -

(∆E(CCBS)HFTZVP(P) + ∆E(CCBS)corrTZVP(P)) (9)

E(S)PBE+D//PBE ) E(S)PBE + Edisp(S) (10)

k(T) ) σkBT

h

QTS(T)

QR(T)exp[-Eq/RT] (11)

Figure 2. The largest system calculated with CCSD(T)/def2-TZVP in thepresent work is the 3T cluster with the overall composition C8H19O4Si2Al(here: adsorbed ethylbenzene). Color codes: oxygen (red), silicon (yellow),aluminum (pink), hydrogen (white), carbon (gray).

J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010 11529

Modeling of Benzene Ethylation over H-ZSM-5 A R T I C L E S

are larger than the experimental values of -398 cm-1 (ref 65)and -360 cm-1 (ref 66), which is also a known characteristicof gradient corrected functionals in general and PBE inparticular.67 However, the difference of -38 cm-1 between theexperimentally observed red-shifts for ethene and benzeneadsorption is predicted well by the calculated value (-38 cm-1)leading us to conclude that the calculated adsorption complexesare reasonable representations of the precursors at the acid site.

3.1.2. Cluster Model Convergence. Figure 4 shows the resultsof the single-point MP2 and PBE cluster calculations. Theadsorption energies do not show a systematic behavior as afunction of the cluster size. Up to a certain cluster size theadsorption energies become more negative and then lessnegative. Neither the size of the cluster at which the energieshave their lowest value nor the magnitude by which the energiesincrease again seems to be predictable. If, however, the high-level correction is plotted, that is, the difference between MP2and PBE adsorption energies, ∆E(C)MP2 - ∆E(C)PBE, decreasingcurves are obtained that converge asymptotically (see Figures5 and 6). With the exceptions of ethene physisorption andchemisorption (ethoxide formation), the decay is monotonic.These adsorption energy differences are used for fitting theanalytical expression given in eq 6. The high-level corrections∆Ẽ(S)high are summarized in row 2 of Table 1. Additionalcalculations addressing the influence of the cluster terminationand the size of the unit cell from which the clusters were cutout, revealed that the high-level corrections are insensitivetoward these issues (see section S.7 of the Supporting Informa-tion for a detailed discussion).

3.1.3. Extrapolation to the Complete Basis Set Limit. TheCBS-limit corrections evaluated according to eq 9 for 18Tcluster models (16T in case of ethene-benzene coadsorption)are listed in the third row of Table 1.

3.1.4. CCSD(T) Corrections. The CCSD(T) corrections arelisted in the fourth row of Table 1. Compared to the previous

application of the hybrid scheme to the protonation of isobutenein zeolite ferrierite,9 the CCSD(T) corrections computed in thepresent work are always positive. It should be noted that theCCSD(T) correction as defined above contains two contribu-tions, the difference between CCSD(T) and canonical MP2adsorption energies which are obtained along the CCSD(T)calculations and the difference between canonical MP2 resultsand the RI-MP2 results. The latter difference is less or equal to2 kJ/mol. Consequently, the “real” CCSD(T) corrections to theMP2:DFT adsorption energies are less than 8%. This issomewhat larger than in former applications of the hybridscheme9,23 and might be attributed to the known tendency ofMP2 to overrate electron correlation effects in unsaturatedsystems and complexes.68 Therefore, the calculation of CCSD(T)corrections is an essential part of the hybrid approach in thepresent case.

3.1.5. Final Estimates of Adsorption Energies andComparison with Experimental Data. The final estimates of thehybrid MP2:DFT adsorption energies are obtained from the sumof the PBE energy, the high-level correction extrapolated to theperiodic limit, the complete basis set limit (CBS) correction,and the CCSD(T) corrections, eq 3. Table 1 summarizes all ofthese contributions. The differences between the final estimatesand the PBE results are substantial. For the physisorptionstructures 1-4 and 6-7 they are between 6.2 and 13.4 kJ/molper CHn unit. For ethylbenzene (3) and the coadsorption ofethene and benzene (4) the total difference is as large as 100kJ/mol. There are not only substantial quantitative changes, butalso qualitative ones. PBE predicts the counterintuitive sequenceethene > benzene > ethylbenzene for the adsorption strength,whereas our final estimates reverse this sequence.

Before we compare with experiment, we will make an attemptto determine the uncertainty of our final estimates. Differentchoices of the unit cell size in the DFT/plane-wave structureoptimization lead to differences of up to around 5 kJ/mol inthe adsorption energy. The use of DFT/plane-wave structuresinstead of reoptimizing the structures at the hybrid MP2:DFTlevel may lead to changes of up to 10 kJ/mol, as we learn fromcomparing DFT and DFT+D optimization results.10 Additional

(65) Spoto, G.; Bordiga, S.; Ricciardi, G.; Scarano, D.; Zecchina, A.;Borello, E. J. Chem. Soc. Faraday Trans. 1994, 90, 2827–2835.

(66) Mukti, R. R.; Jentys, A.; Lercher, J. A. J. Phys. Chem. C 2007, 111,3973–3980.

(67) Tuma, C.; Boese, A. D.; Handy, N. C. Phys. Chem. Chem. Phys. 1999,1, 3939–3947. (68) Schwabe, T.; Grimme, S. J. Phys. Chem A 2009, 113, 3005–3008.

Table 1. Adsorption Energies Obtained Using the Hybrid MP2:DFT Scheme and PBE+D Adsorption Energies at the PBE OptimizedStructures As Predicted by the Parameters of Grimme13 a

1 2 3 4 5 6 7b

∆E(S)PBE -31.5 -24.0 -16.6 -40.7 -53.5 -2.0 -4.2∆Ẽ(S)high -26.7c -76.2d -118.3 -122.6 -27.5 -95.8 -20.5∆E(C18)MP2CBS 5.8 14.2 13.8 14.8e 12.9 11.7 7.7∆E(C3)CCSD(T)f 4.1 5.5 6.1 7.5 6.9 3.9 0.5∆Ẽ(S)final estimate -48.3 -80.5 -115.1 -141.0 -61.3 -82.2 -16.5difference to PBE -16.8 -56.5 -98.5 -100.3 -7.7 -80.2 -12.3

∆E(S)ZPV 1.4 -0.2 2.8 6.4 10.5 4.1 -1.9∆H(S)298 - ∆E0(S)PBEg 1.1 2.6 2.3 3.9 -2.6 3.0 4.7∆H(S)653 - ∆E0(S)PBEh 6.5 8.5 7.2 14.2 0.3 8.5 11.6

∆E(S)D//PBE -29.2 -63.0I -100.8 -97.7 -33.7 -73.6 -18.8∆E(S)PBE+D//PBE -60.6 -86.9 -117.4 -138.3 -87.3 -75.6 -23.0

∆E(C18)highDFT+D 1.2 -11.4 -12.1 -10.9e 3.2 -11.7 -2.7∆E(S)final estimateDFT+D -49.5 -78.7 -109.6 -126.9 -64.3 -71.7 -17.5

a Zero-point vibrational energies and thermal contributions to adsorption enthalpies are also included. Energies are reported in kJ/mol. b Adsorption inchannel intersection. c This values remains the same for Al-O-Si(OH)3 instead of Al-O-H termination. d -76.5 kJ/mol for the second set of unit cellparameters. e For 16T cluster. f Difference between CCSD(T) and RI-MP2 adsorption energies on a 3T cluster. g Contribution to enthalpy at 298 K(∆E0(S)PBE is the ZPVE corrected adsorption energy). h Contribution to enthalpy at 653 K (∆E0(S)PBE is the ZPVE corrected adsorption energy). I -60.9kJ/mol for the second set of unit cell parameters.

11530 J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010

A R T I C L E S Hansen et al.

uncertainties are introduced by the fitting procedure and theextrapolation to the CBS limit. The maximum deviation betweenthe reference data points and the fitted values are 3.7 kJ/mol(see Table S.6 of the Supporting Information). Following ref23 we estimate the uncertainty in the CBS limit to (2.5 kJ/mol. As a conservative assumption, a range of (10 kJ/molaccounts for all uncertainties of our methodology, in agreementwith previous applications of the hybrid MP2:DFT approach.9,23

Table 2 compares adsorption enthalpies calculated from ourfinal estimates by adding the zero-point vibrational energies andthermal corrections evaluated from PBE frequencies withavailable experimental data. Experimental heats of adsorptionfor ethene in acidic H-ZSM-5 are not available directly. Thecalculated enthalpy of adsorption at the acid site, -45.8 kJ/mol, is compared with the experimental value for an H,Na-Yzeolite.69 Adsorption enthalpies in the aluminum-free analogue,silicalite-1, are ranging from -24 to -31 kJ/mol (see ref 70

and references therein). For ethene, adsorption in the channelintersections is not most favorable. Additional PBE+D//PBEcalculations for two representative adsorption sites in thesinusoidal and straight channel yield -32.9 and -30.0 kJ/mol,respectively. If the difference of 9.9 kJ/mol between thesinusoidal channel and the intersection is added to the finalestimate for the channel intersection, an ∆H value of -23.6kJ/mol is obtained.

For benzene adsorption in H-ZSM-5, the most reliableexperimental result (calorimetry, ref 71) is -63.6 kJ/mol. Otherresults are ranging from -59.0 to -69.0 kJ/mol (see ref 24and references therein) indicating an uncertainty range of (5

(69) Cant, N. W.; Hall, W. K. J. Catal. 1972, 25, 161–172.

(70) Jakobtorweihen, S.; Hansen, N.; Keil, F. J. Mol. Phys. 2005, 103, 471–489.

(71) Thamm, H.; Jerschkewitz, H.-G.; Stach, H. Zeolites 1988, 8, 151–153.

(72) Niessen, W.; Karge, H. G.; Jozefowicz, L. Stud. Surf. Sci. Catal. 1993,80, 475–481.

(73) Thamm, H.; Stach, H.; Fiebig, W. Zeolites 1983, 3, 95–97.

Figure 3. Adsorbed ethene, benzene, and ethylbenzene (1-3), coadsorbed ethene and benzene (4), ethoxide (5), benzene adsorbed next to ethoxide (6), andethene adsorbed in the channel intersection of all-silica MFI (7).

J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010 11531

Modeling of Benzene Ethylation over H-ZSM-5 A R T I C L E S

kJ/mol. The experimental enthalpy of adsorption for ethylben-zene, (-87 kJ/mol, ref 72), is 23 kJ/mol more negative thanthat for benzene.

The calculated adsorption enthalpies for ethene, isobutene(refs 9, 22), benzene and ethylbenzene are more negative by 8,10-14, 14, and 23 kJ/mol, respectively, than the experimentalvalues. This small (2-4 kJ/mol per CHn unit) and systematicoverestimation of the strength of the binding to the Brønsted

acid site we ascribe to remaining uncertainties in our methodol-ogy. Moreover, our calculated values refer to one particular sitechosen such that the adsorbate can maximize its interaction withthe acid site on the zeolite surface (channel intersection),whereas the experimental sample contains a distribution of sitesover different crystallographic positions, and these sites are notordered into unit cells. Compared to previous B3LYP T33cluster results for ethene, benzene, and ethylbenzene,24 whichwere respectively 3, 24, and 48 kJ/mol too small (in absoluteterms) our final estimate adsorption enthalpies are substantiallyimproved.

3.2. Reaction Steps. 3.2.1. Periodic DFT Structure Optimiza-tion. The first row of Table 3 shows the PBE energy barriersfor all forward and reverse reactions obtained with the UC1 setof cell parameters. The energy barriers for the reverse reactions‘1s, rev’ and ‘2s(2), rev’ were calculated with respect to structure3 shown in Figure 3. The energy barrier for the reverse reaction‘2s(1), rev’ was calculated with respect to structure 5 shown inFigure 3. The size of the unit cell only affects the second barrierof the two-step scheme by 6.1 kJ/mol. The influence of the unitcell size on ZPVE and thermal contributions is below 2 kJ/mol(see section S.6.2 of the Supporting Information for a detaileddiscussion). The frequency analysis revealed the presence ofexactly one imaginary frequency for all transition structures,which are illustrated in Figure 7.

3.2.2. Cluster Model Convergence. Figure 8 shows the clustersize dependence of the apparent energy barriers, Eappq (C), forforward and reverse reaction steps obtained from single-pointMP2 and PBE cluster calculations. Note that for the first stepof the two-step mechanism an apparent energy barrier for thereverse reaction is not required because the intrinsic barrier iscalculated from the apparent energy barrier of the forwardreaction and the reaction energy for ethoxide formation fromthe unloaded zeolite cluster and ethene in the gas phase. Forthe second step of the two-step mechanism we calculated theapparent energy barrier of the forward reaction with respect tothe unloaded zeolite cluster and ethene and benzene in the gasphase and not with respect to ethoxide and benzene in the gasphase because a better fit of the MP2-PBE difference wasachieved for the former choice. In contrast to the adsorptionenergies, the apparent energy barriers decrease uniformly withincreasing cluster size. However, even for the largest cluster

Figure 4. Adsorption energies obtained from single-point energy calcula-tions on cluster models of increasing size. (a) MP2/TZVP(P) results. (b)DFT (PBE/QZVP) results. The periodic model limit is included forcomparison.

Figure 5. Differences in adsorption energies between MP2 and PBE (filledand partly filled symbols) and dispersion contributions to the adsorptionenergies as predicted by the parameter set published by Grimme13 (opensymbols). Extrapolations to the full periodic limit are also included.

Figure 6. Differences in adsorption energies between MP2 and PBE (filledsymbols) and dispersion contributions to the adsorption energies as predictedby the parameter set published by Grimme13 (open symbols). Extrapolationsto the full periodic limit are also included.

11532 J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010

A R T I C L E S Hansen et al.

they have not converged and in most cases differ substantiallyfrom the periodic limit (see Figure 8b). If the difference between

the MP2 and PBE apparent energy barriers is plotted, decayingcurves are obtained that converge asymptotically and can befitted to the analytical expression given in eq 6 (see Figure 9).

The high-level corrections for the intrinsic energy barriershave been obtained by taking the difference between the high-level corrections for the apparent energy barriers and the high-level corrections of the corresponding adsorbate complexes.These energies are listed in the second row of Table 3. ThePBE intrinsic barriers for the one-step scheme and for the firststep of the two-step scheme are substantially increased by thehigh-level corrections. For the second barrier of the two-stepscheme the high-level correction is significantly smaller.

3.2.3. Extrapolation to Complete Basis Set Limit. The com-plete basis set limit correction for each intrinsic energy barrierhas been determined as the difference between the CBS-limitcorrection for the apparent energy barrier and the CBS-limitcorrection for the formation of the corresponding adsorptioncomplex. Depending on the reaction channel, different frag-mentations of the system have been used in the counterpoisecalculation (see section S.3 of the Supporting Information fordetails). The CBS limit corrections for the intrinsic energiesbarrier are listed in the third row of Table 3.

3.2.4. CCSD(T) Corrections. CCSD(T) corrections are listedin the fourth row of Table 3. For the forward reaction steps thedifferences between CCSD(T) and MP2 are very small (+0.5,-1.9, and -1.0 kJ/mol) showing that MP2 yields energy barriersof CCSD(T) quality. For the reverse reactions larger CCSD(T)corrections are obtained (-12.8, -4.7, and -11.0 kJ/mol) which

Table 2. Comparison of Calculated Adsorption Energies and Enthalpies with Experiments (in kJ/mol)

PBE+D final estimate

-∆E -∆E -∆H obsd

ethene MFI, sinusoidal channel 32.9 (23.6)g 24-31aMFI, intersection 23.0 16.5 13.7H-MFI, Al12-O20(H)-Si3 60.6 48.3 45.8 38b

benzene H-MFI, Al12-O20(H)-Si3 86.9 80.5 78.1 63.6c64 ( 5d

ethylbenzene H-MFI, Al12-O20(H)-Si3 117.4 115.1 110.0 87 ( 5disobutene FER 65.7i (48.1)h 49e

isobutene H-FER 90.5k 77.2k 72.9k 59-63f

a See ref 70 for original references. b H,Na-Y zeolite, ref 69. c Calorimetry, 1 molecule/unit cell, Si/Al ) 86, ref 71. d 2 molec/uc, Si/Al ) 34, butlarge amounts of extraframework Al, ref 72. e But-1-ene in MFI (silicalite-1), ref 73. f Estimated, see ref 9. g Estimated from PBE+D difference tointersection and the final estimate for the latter. h Estimated from PBE+D difference to H-FER and the final estimate for the latter. i Reference 10.k References 9, 22.

Table 3. Intrinsic Energy Barriers Obtained Using the Hybrid MP2:DFT Scheme and PBE+D Intrinsic Energy Barriers at the PBE OptimizedStructures As Predicted by the Parameters of Grimme13 a

1s 1s, rev 2s(1) 2s(1), rev 2s(2) 2s(2), rev

Eq(S)PBE 84.3 173.1 91.6 113.7 95.9 169.9∆Ẽq(S)high 43.9 58.1 39.3 40.2 7.4 21.1∆Eq(C16)MP2CBS 1.0 2.5 0.6c -6.5c 0.2 10.4∆Eq(C3)CCSD(T)b 0.5 -12.8 -1.9 -4.7 -1.0 -11.0Ẽq(S)final estimate 129.7 220.9 129.7 142.7 102.5 190.3difference to PBE 45.4 47.8 38.1 29.0 6.6 20.4

∆Eq(S)ZPV -4.8 -14.7 -2.4 -11.4 -5.0 -6.7Hq(S)653 - E0q(S)PBEd -7.7 -0.4 -8.6 -2.5 -3.8 -1.9

∆Eq(S)D//PBE -14.4 2.1 -7.5 -3.0 -22.7 -15.9Eq(S)PBE+D//PBE 69.9 175.3 84.1 110.7 73.2 154.0

∆Eq(C16)highDFT+D 56.0 62.7 53.9 51.6 35.1 42.2Eq(S)final estimateDFT+D 127.3 227.7 136.7 151.2 107.5 195.5

a Zero-point vibrational energies and thermal contributions to enthalpy barriers are also included. Energies are reported in kJ/mol. b Differencebetween CCSD(T) and RI-MP2 energy barriers on a 3T cluster. c For 18T cluster. d Contribution to enthalpy at 653 K (E0q(S)PBE is the ZPVE-correctedenergy barrier).

Figure 7. Transition-state structures for one-step and two-step alkylations.

J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010 11533

Modeling of Benzene Ethylation over H-ZSM-5 A R T I C L E S

indicate an overstabilization of the reaction product, adsorbedethylbenzene, by MP2.

3.2.5. Final Estimate for Energy Barriers. Table 3 shows thefinal estimate for intrinsic energy barriers which are obtainedfrom the PBE energy barrier, the high-level corrections ex-trapolated to the periodic limit, the basis set limit corrections,and the CCSD(T) corrections, see eq 3. For the one-step scheme,the energy barrier is 129.7 kJ/mol. For the two-step scheme weobtained 129.7 kJ/mol for the first step and 102.5 kJ/mol for

the second step. While the energy barrier for the one-stepscheme determined in the present study differs only slightlyfrom that determined in our earlier B3LYP cluster study (Eq )123.2 kJ/mol)24 there are significant deviations for the two-stepscheme. For the first step the final estimate barrier is 24 kJ/molhigher, while it is 13 kJ/mol lower for the second step. In thesecalculations of energy barriers for the alkylation, the hybridMP2:DFT results are affected by the same type of uncertaintiesas the calculations of adsorption energies. Therefore, anuncertainty range of (10 kJ/mol is expected.

The final estimates of the present study provide a significantimprovement in the theoretical description of benzene alkylationover H-ZSM-5, if we keep in mind that the intrinsic barriersfrom the DFT cluster study strongly depend on the cluster size.This is the result of a partial compensation of two types of errorsin plane PBE:23 missing dispersion which results in too highbarriers and self-interaction correction errors which result insystematically too low barriers. Because the former dependsmuch more on the cluster size than the latter, the extent of thecompensation and the resulting barriers strongly depend on thecluster size (see also section 3.3).

Figure 10 compares the final estimate potential energy profilewith the PBE profile and the B3LYP profile for the T33 clustercalculated previously.24 The final estimate profile is shifted downsubstantially relative to the DFT profiles. More importantly thisshift is different for reactants and transition states due to differentself-interaction errors.

3.3. DFT+D. 3.3.1. PBE+D//PBE Results. Figures 5 and 6show the dispersion contributions to the adsorption energiescalculated for different cluster sizes according to eq 6 with thetransferable parameters of Grimme,13 (open symbols). Thevalues for the periodic structures (number of T atoms ) ∞) arealso shown in Table 1 (row 9). Row 10 of Table 1 contains thetotal PBE+D//PBE adsorption energies (eq 10) which show asubstantial improvement compared to plane PBE results. Thedeviation from the final estimate based on our hybrid MP2:DFT results is small, -6.4, -2.3, +2.7, and +6.6 kJ/mol (-8,-2, +2, and +8%) for 2, 3, 4, and 6, respectively, i.e. for allphysisorption steps except ethene. For ethene physisorption onthe silica wall (7), on the Brønsted site (1), and for ethoxideformation (5), PBE+D overestimates the binding energies by6.5, 12.4, and 26 kJ/mol, in agreement with previous work forisobutene on H-FER.10,22

For energy barriers the dispersion contributions and the totalPBE+D energies, evaluated as difference between the reactantsand the transition structures, are shown in rows 9 and 10 ofTable 3. Compared to our final estimates for the hybrid MP2:PBE results, the PBE+D barriers, which are affected by the

Figure 8. Apparent energy barriers for the one- and two-step alkylationsobtained from single-point energy calculations on cluster models ofincreasing size. (a) MP2/TZVP(P) results. (b) DFT (PBE/QZVP) results.The periodic model limit is included for comparison.

Figure 9. Differences between the two series of apparent energy barriersshown in Figure 8 and extrapolation to the periodic limit.

Figure 10. Potential energy profiles for the alkylation of benzene obtainedwith different methods.

11534 J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010

A R T I C L E S Hansen et al.

self-interaction correction error only, are too low by 59.8, 45.6,and 29.3 kJ/mol for 1s, 2s(1) and 2s(2) steps, respectively. Thisis in the range of 12-62 kJ/mol by which PBE barriers fordifferent types of reactions are known to be too low.11 The planePBE barriers are too low by 45.4, 38.1, and 6.6 kJ/mol,respectively, due to partial compensation between missingdispersion (-14.4, -7.5, and -22.7 kJ/mol, row 9 in Table 3)and the self-interaction correction error.

3.3.2. Discussion. In terms of model chemistry the conclusionfrom this and previous studies22,23 is that the PBE+D modelmaintains the performance of the PBE model also in cases forwhich dispersion is important. That means that PBE+D willshow the same underestimation of barriers and the sameoverstabilization of polar structures as PBE. An improvementwould be possible with density functionals that have a smallerself-interaction correction error such as hybrid functionals.

The B3LYP+D model is expected to yield adsorptionenergies that are close to our hybrid MP2:PBE+∆CCSD(T)model and to yield improved results for reaction barriers.Reference 11 reports a range of 6-36 for barrier errors withB3LYP compared to 12-62 kJ/mol with PBE. The problem isthat calculations with hybrid functionals applying periodicboundary conditions would not be feasible for zeolite catalystsbecause the unit cells are large and symmetry is low or absent.A possibility is a hybrid B3LYP+D(cluster):PBE+D(pbc) +∆CCSD(T) scheme, which would maintain the performance ofthe B3LYP+D model also for extended systems representedby large unit cells and periodic boundary conditions.

The most effective use of PBE+D calculations is probablyas low level method in a hybrid scheme. The most expensivepart of our hybrid MP2/CBS:PBE scheme is the evaluation ofthe high-level correction, eq 1, which requires MP2 calculationsfor different cluster sizes. Figures 5 and 6 show that thedispersion term, calculated with the transferable Grimmeparameters, has the same dependency on the cluster size. Thismeans that the high-level correction calculated for PBE+D asthe low level method, i.e.

depends only weakly on the cluster size in most cases, see Figure11, which suggests a hybrid MP2/CBS(cluster):DFT+D(pbc)+ ∆CCSD(T) approach. Such a scheme would avoid any fitting

and the high-level correction would be evaluated for one clustersize CMP2 only.

Figure 11 suggests that in most cases clusters in the 16T-18Tsize region would be sufficient. Since MP2/CBS results for T18have not been calculated for all systems, we use here the T18results if available and T16 in the other cases to calculate∆E(C)highDFT+D and ∆E(S)final estimateDFT+D according to eqs 12 and 13.The results for adsorption energies and intrinsic barriers areshown in the bottom rows of Tables 1 and 3, respectively. Thedeviation from the final estimate adsorption energies based onour MP2:DFT results is small for 1, 2, 3, 5 and 7 (-1.2, +1.8,+5.5, -3.0, and -1.0 kJ/mol), i.e. for all steps for which thedifference between MP2 and DFT+D adsorption energies doesnot show large variations beyond the T18 cluster (see Figure11). Especially the reaction energies for 1, 5, and 7, evaluatedwith eq 13, deviate significantly less from the MP2:DFT finalestimates than the PBE+D results, showing that eq 13 offersan attractive approach to improve PBE+D results with reason-able computational costs. The deviation of the intrinsic barrierscalculated by means of eq 13 from the final estimates is alsosmall (-2.3, +7.0, and +5.9 kJ/mol) for 1s, 2s(1) and 2s(2),i.e. less than 6%. This remarkable agreement results from errorcompensation because the MP2-DFT+D results evaluated forthe T16 cluster for both reactant states and apparent barriersshow similar deviations from the extrapolations to their periodiclimits.

3.4. Rate Coefficients for Elementary Steps and Com-parison with Experimental Data. Enthalpy barriers are obtainedfrom our final estimate energy barriers by adding the zero-pointvibrational energies and thermal corrections (rows 7 and 8 inTable 3, respectively), both calculated from PBE frequencies.The intrinsic energy and enthalpy barriers have to be convertedinto apparent activation energies before they can be comparedto experimental data.

Rate coefficients for all elementary reaction steps werecalculated according to eq 11. As is justified in section S.5 ofthe Supporting Information, the partition functions of reactantand transition state were evaluated from vibrational contributionsonly. For the one-step mechanism the reaction path symmetry

Figure 11. Differences between MP2 and PBE+D results for adsorption energies and apparent energy barriers as function of cluster size.

∆E(C)highDFT+D ) ∆E(C)MP2 - ∆E(C)DFT+D (12)

∆E(S)final estimateDFT+D ) ∆E(S)DFT+D + ∆E(CMP2)high

DFT+D +

∆E(CMP2)MP2CBS + ∆E(CCC)CCSD(T) (13)

J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010 11535

Modeling of Benzene Ethylation over H-ZSM-5 A R T I C L E S

number was set to σ ) 12 in order to account for the fact thateach of the two C-atoms of ethene can react with each of thesix C-atoms of benzene. The rate coefficient is therefore largerby a factor of 12 compared to the single-event rate coefficientobtained if all C-atoms were distinguishable. For the first stepof the two-step mechanism we used σ ) 2, while for the secondstep σ ) 6 was employed. The rate coefficients obtained arelisted in Table 4 for relevant reaction temperatures. It shouldbe noted that the preexponential factors determined in the presentwork are similar to those obtained in our cluster study24 (seeTable 5). The largest deviation is observed for the ethoxideformation. For this process the preexponential factor obtainedin the present work is higher by a factor of 4 compared to thevalue obtained in our cluster study. The changes in the ratecoefficients compared to those in our cluster study are thereforemostly due to the differences in the calculation of intrinsicenergy barriers as well as the consideration of reaction pathsymmetry numbers.

Experimentally determined rate data for the alkylation ofbenzene depend on a number of items in addition to the intrinsicrate coefficients. These are in particular the external conditionssuch as pressure, temperature, and gas-phase composition butalso the particle size and shape. All of these factors determinethe average concentration of precursor states inside the zeolitechannel system and consequently the effective rate of reactionvia

In this equation, r denotes the overall rate of reaction in molkg-1 s-1, ki are the intrinsic rate coefficients for forward andreverse reactions, and 〈Npre,i〉 are the average concentrations ofprecursors for forward and reverse reactions, respectively, inmol kg-1. In a previous publication27 we have introduced aphenomenological model that relates the external conditions(temperature, pressure, and gas phase composition) to theconcentration of precursor states based on the multicomponentadsorption behavior of the ethene-benzene-ethylbenzenemixture as well as on the distribution of these species inside

the zeolite channel system. As a result, the rates calculated bymeans of eq 14 can be compared to experimental data.Alternatively we can use turnover frequencies obtained from

where r is the rate of reaction according to eq 14 and cH+ is theconcentration of acid sites in mol kg-1, respectively. Fromcalculated turnover frequencies at different temperatures we canobtain the apparent activation energy by means of an Arrheniusplot. Figure 12 shows simulated Arrhenius plots at 2.5 baroverall gas pressure, and a fixed benzene to ethene ratio of 5:1.For the one-step scheme the average concentrations 〈Npre,1〉 ineq 14 at 603 and 653 K are 1.73 × 10-3 and 7.31 × 10-4molecules per unit cell, respectively.27 Note that 〈Npre,-1〉 wasessentially equal to zero in the calculations, as virtually noethylbenzene was present in the gas phase. Some experimentalpoints74 are also included in Figure 12. They were determinedin a mesoporous and a conventional ZSM-5 sample, respec-tively. The difference in the activity among the two sampleswas attributed to diffusional limitation in the case of the

Table 4. Intrinsic Rate Coefficients for the One-Step and Two-Step Mechanisms

T (K)

reaction constant 603 653 703

HOZ(C2H4 + C6H6) f HOZ(C8H10) (1s)k1, s-1 5.04 × 100 3.28 × 100 1.64 × 102k-1, s-1 3.85 × 10-6 9.68 × 10-5 1.54 × 10-3

HOZ(C2H4) f C2H5OZ (2s(1))k1, s-1 8.87 × 100 5.91 × 101 3.00 × 102k-1, s-1 4.92 × 102 3.81 × 103 2.22 × 104

C2H5OZ(C6H6) f HOZ(C8H10) (2s(2))k1, s-1 2.85 × 104 1.29 × 105 4.75 × 105k-1, s-1 4.40 × 10-5 7.65 × 10-4 8.89 × 10-3

Table 5. Preexponential Factors of Elementary Steps in s-1

T (K)

reaction 603 653 703

HOZ(C2H4 + C6H6) f HOZ(C8H10) (1s)ref 24 2.60 × 1010 2.46 × 1010 2.35 × 1010this work 2.78 × 1010 2.68 × 1010 2.60 × 1010

HOZ(C2H4) f C2H5OZ (2s(1))ref 24 1.11 × 1011 1.07 × 1011 1.03 × 1011this work 4.75 × 1011 4.53 × 1011 4.34 × 1011

C2H5OZ(C6H6) f HOZ(C8H10) (2s(2))ref 24 1.41 × 1012 1.47 × 1012 1.53 × 1012this work 1.33 × 1012 1.36 × 1012 1.39 × 1012

r ) k1〈Npre,1〉 - k-1〈Npre,-1〉 (14)

TOF ) r/cH+ (15)

Figure 12. Experimental and simulated Arrhenius plots for the alkylationof benzene at 2.5 bar and a benzene to ethene ratio in the gas phase of 5:1.The experimental data were obtained for mesoporous (9) and conventional(b) H-ZSM-5.74 The simulated turnover frequencies are plotted for the one-step mechanism, the two-step mechanism, and for the sum of both.

11536 J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010

A R T I C L E S Hansen et al.

conventional zeolite sample. It should be noted, though, thatdifferences in the multicomponent adsorption equilibriumbetween the two samples might contribute to the observeddifferences in activities in addition to the effects of intraparticlediffusion. Therefore, the experimental points shown in Figure12 define a range of possible turnover frequencies for benzenealkylation over H-ZSM-5 samples. The simulated curves forthe one- and two-step schemes both underestimate the experi-mental data. An overall turnover frequency obtained from thesummation of the two contributions75 is also included in Figure12. The positions of the simulated Arrhenius plots depend onthree factors which are the following: first, our final estimatesfor the intrinsic energy barriers; second, our estimates of theintrinsic preexponential factors; and third, the estimation ofprecursor concentrations by means of our phenomenologicalmodel.27 Table 6 compares apparent Arrhenius parameterscalculated from our final estimates with Arrhenius parametersdetermined from experimental data. The calculated apparentactivation energies of the two reaction mechanisms, 66.1 and112.0 kJ/mol differ substantially. Only the apparent activationenergy of the one-step scheme agrees with the experimentaldata within the uncertainty limit of our calculations. While thiscould lead to the conclusion that our results for the two-stepscheme are not correct, it has to be kept in mind that the energybarrier for the two-step scheme was calculated assuming thatethene enters an empty intersection. This assumption, though,is not correct since an excess of benzene was used in theexperiments reported in ref 74. As a result, the probability ofethene finding an unoccupied intersection is lowered consider-ably because benzene adsorbs much more strongly than ethenein the channel intersection. Therefore, it is likely that under suchconditions the two-step mechanism is much less relevant thanthe one-step scheme because any protonated ethene would reactwith benzene directly instead of forming a surface ethoxide.Therefore, we limit the comparison with experiments to the one-step mechanism. Under the conditions of a significant excessof benzene in the gas phase the apparent activation energy canalso be estimated directly (i.e., without using our continuummodel27) from our calculated adsorption energies and energybarriers reported in Tables 1 and 3. Then the reaction can beassumed to be intrinsic with respect to benzene but apparentwith respect to ethene. As a result we can add the difference ofthe adsorption enthalpies for reaction 4 and 2 at 653 K (-120.5and -72.2 kJ/mol) to the intrinsic enthalpy barrier at 653 K(117.2 kJ/mol) to obtain the apparent enthalpy barrier (69.0 kJ/mol). The apparent activation energy is then obtained afteradding RT. The result, 74.4 kJ/mol, is in reasonable agreementwith the value obtained from the continuum model. Thedifference of 8 kJ/mol indicates the importance of an accuratecalculation of the precursor concentration.

One reason for underestimation of the experimental turnovernumbers might be connected with uncertainties in the estimationof precursor concentrations. An error range is hard to quantifybecause reliable high temperature adsorption data are notavailable to test whether force fields parametrized at ambienttemperature are still valid at reaction temperature. Moreover ithas been shown that adsorption can be very sensitive to smalldeviations in the crystal structure of the zeolite under study,especially at low pressures.76 However, taking into account theresults of the latter study, it is unlikely that the uncertaintiesincluded in the estimation of the precursor concentration areresponsible for the 1 order of magnitude deviation. The secondreason is most likely connected to the calculation of intrinsicpreexponential factors by means of the harmonic approximationwhich faces its limits at temperatures as high as needed forhydrocarbon reactions in zeolites. These limitations can beovercome by taking into account entropy effects beyond theharmonic approximation, for example by means of transitionpath sampling.77 Finally it should be noted that the experimentaldata are also subject to uncertainties, the estimation of whichis beyond the scope of the present study.

4. Conclusion

A hybrid MP2:DFT + ∆CCSD(T) approach was used tostudy elementary adsorption and reaction steps involved in thealkylation of benzene with ethene over H-ZSM-5. The dispersionenergy contributes substantially to the final estimates for theadsorption energies, leading to a reversal of the stabilitysequence predicted by plane-wave PBE calculations for theadsorption of ethene, benzene, and ethylbenzene on the Brønstedacid site. Calculated adsorption enthalpies are more negativethan experimental data by 2-4 kJ/mol per CHn unit.

The final estimates for intrinsic energy barriers deviatesignificantly from the plane-wave PBE barriers which aresystematically too low. Intrinsic energy barriers are convertedto apparent activation energies by means of a phenomenologicalmodel based on the multicomponent adsorption equilibrium ofthe ethene-benzene-ethylbenzene mixture.27 Whereas the two-step mechanism is unlikely to occur under the conditions ofthe experiment, the apparent activation energy for the one-stepalkylation (66 kJ/mol) agrees with the experimental data (58-76kJ/mol) within the uncertainty limit of our calculations ((10kJ/mol). Comparison with the intrinsic barrier (129.7 kJ/mol)shows that under the experimental conditions the reaction isessentially intrinsic with respect to benzene, but apparent withrespect to ethene. The calculated turnover frequencies areunderestimated compared to the experimental values which ismost likely due to the harmonic approximation applied in thecalculation of preexponentials. Future improvements requiresampling the anharmonic potential energy surface. Part of theremaining deviations for both barriers and preexponentials canbe ascribed to the fact that our calculations refer to one particularsite in the zeolite in contrast to experimental data that areaverages over a distribution of sites.

As far as methods are concerned, we have shown in this andin previous studies9,21-23 that a reliable description of hydro-carbon reactions in zeolites, in particular, and reactions occurringon a local site in a large chemical system, in general, is only

(74) Christensen, C. H.; Johannsen, K.; Schmidt, I.; Christensen, C. H.J. Am. Chem. Soc. 2003, 125, 13370–13371.

(75) Laidler, K. J. Chemical Kinetics, 3rd. ed.; Harper & Row: New York,1987.

(76) Zimmermann, N. E. R.; Haranczyk, M.; Sharma, M.; Liu, B.; Smit,B.; Keil, F. J. Mol. Simul., submitted.

(77) Bučko, T.; Benco, L.; Dubay, O.; Dellago, C.; Hafner, J. J. Chem.Phys. 2009, 131, 214508–1/11.

Table 6. Comparison of Apparent Arrhenius Parameters Obtainedfrom Final Estimates with Experiments (in kJ/mol and 1/s)

calcd obsd

Eapp Aapp Eapp Aapp

1s 66.1 3.41 × 10358- 2.44 × 104-

2s 112.0 2.09 × 10876 1.38 × 106

total 107.5 9.74 × 107

J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010 11537

Modeling of Benzene Ethylation over H-ZSM-5 A R T I C L E S

possible with a method that includes dispersion, limits the self-interaction correction error, and takes long-range electrostaticeffects into account. The majority of routine DFT calculationscurrently performed and published in these areas do not meetthese requirements and are therefore affected by uncontrolledand sizable errors. In contrast, our hybrid MP2:DFT +∆CCSD(T) method meets all these requirements. In the contextof model chemistry it is a way to maintain the performance ofthe MP2/CBS+∆CCSD(T) model established for molecules alsofor extended systems represented by large unit cells and periodicboundary conditions. The method is by no means limited tohydrocarbon reactions in zeolites but is generally applicable tolarge chemical systems in which dispersion interactions play arole and/or self-interaction correction errors change along thereaction coordinate. Typical examples are adsorption of mol-ecules on, and reactions with, different types of surfaces suchas oxides, semiconductors, graphite and carbon nanotubes, orbiopolymers. It has been successfully used to calculate isothermsfor hydrogen adsorption in metal-organic frameworks,78 andwork on hydrocarbon adsorption on oxide surfaces is inprogress.79 Another area of application is solvation in whichan increasing number of solvent molecules is included in thecluster.

Application of our hybrid approach is not bound to the useof specific codes for the high-level (MP2) and low-level(periodic DFT) method, and when used with fixed geometricstructures that have been obtained at the low level as done here,it does not even require a program that links the codes.Nevertheless, its general use may be hampered by the largenumber of demanding MP2 calculations to be performed andthe need to fit the difference between the MP2 and DFT results(high-level correction). However, this we did only to generatebenchmark data for simpler protocols such as the hybridMP2(cluster):DFT+D(pbc) approach discussed in section 3.3.2.

The latter needs a DFT code with some means of includingdispersion and periodic boundary conditions. A stand-aloneimplementation of the Grimme term that can be combined withperiodic DFT codes is freely available.10 This DFT+D code isused to optimize a structure. For the structure obtained, a clustermodel needs to be defined on which MP2 single-point calcula-tions are performed by any MP2 code available. Special QM:QM coupling software with periodic boundary conditions80 isavailable from two laboratories10,21,81,82 but is only needed ifthere is a reason to improve the DFT+D structures and tooptimize on the hybrid MP2(cluster):DFT+D(pbc) potentialenergy surface.

Acknowledgment. The present work was supported by theDeutsche Forschungsgemeinschaft (DFG) in priority program SPP1155 and the Methane Conversion Cooperative supported by BP.Computations were partly carried out at the Norddeutscher Verbundfür Hoch- und Höchstleistungsrechnen (HLRN). N.H. acknowledgesTomáš Bučko for providing an implementation of the improveddimer method into VASP.

Supporting Information Available: Possible location of acidicsite in H-ZSM-5; description of procedure for extrapolation tothe complete basis set limit and details of BSSE calculationsfor transition states and intermediates; discussion of differentapproaches to calculate the reactant partition function; influenceof unit cell parameters on PBE energies; additional dataillustrating the cluster size dependence of adsorption energiesand energy barriers; fit parameters; energies and Cartesiancoordinates of stationary points; complete refs 55 and 82. Thismaterial is available free of charge via the Internet at http://pubs.acs.org.

JA102261M

(78) Sillar, K.; Hofmann, A.; Sauer, J. J. Am. Chem. Soc. 2009, 131, 4143–4150.

(79) Tosoni, S.; Sauer, J. Manuscript in preparation.

(80) Sauer, J.; Sierka, M. J. Comput. Chem. 2000, 21, 1470–1493.(81) Sierka, M.; Sauer, J. J. Chem. Phys. 2000, 112, 6983–6996.(82) Sherwood, P.; et al. J. Mol. Struct. (THEOCHEM) 2003, 632, 1–28.

11538 J. AM. CHEM. SOC. 9 VOL. 132, NO. 33, 2010

A R T I C L E S Hansen et al.

Click here to load reader

Embed Size (px)

Recommended